# Electronic Supplementary Material (ESI) for CrystEngComm.
# This journal is © The Royal Society of Chemistry 2017

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_jli245_final
_database_code_depnum_ccdc_archive 'CCDC 1573595'
_audit_update_record             
;
2017-09-10 deposited with the CCDC.
2017-12-01 downloaded from the CCDC.
;

_audit_creation_date             2016-03-28T15:31:03-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'

#----------------------------------------------------------------------------#
#                   CHEMICAL INFORMATION                                     #
#----------------------------------------------------------------------------#

_chemical_name_systematic        'potassium manganese(II) oxalatophosphite '
_chemical_formula_sum            'C2 H6 K2 Mn2 O12 P2'
_chemical_formula_weight         472.09

#----------------------------------------------------------------------------#
#                   UNIT CELL INFORMATION                                    #
#----------------------------------------------------------------------------#

_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_H-M   'P 63/m'
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'x-y, x, z+1/2'
'-y, x-y, z'
'-x, -y, z+1/2'
'-x+y, -x, z'
'y, -x+y, z+1/2'
'-x, -y, -z'
'-x+y, -x, -z-1/2'
'y, -x+y, -z'
'x, y, -z-1/2'
'x-y, x, -z'
'-y, x-y, -z-1/2'

_cell_length_a                   9.7371(2)
_cell_length_b                   9.7371(2)
_cell_length_c                   22.4924(5)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_volume                     1846.82(7)
_cell_formula_units_Z            6
_cell_measurement_temperature    100(2)
_cell_measurement_reflns_used    7232
_cell_measurement_theta_min      2.402
_cell_measurement_theta_max      28.095

#----------------------------------------------------------------------------#
#                   CRYSTAL INFORMATION                                      #
#----------------------------------------------------------------------------#

_exptl_crystal_description       prism
_exptl_crystal_colour            pink
_exptl_crystal_size_max          0.2689
_exptl_crystal_size_mid          0.0834
_exptl_crystal_size_min          0.0726
_exptl_crystal_density_diffrn    2.547
_exptl_crystal_density_method    flotation
_exptl_crystal_density_meas      2.53(4)
_exptl_crystal_F_000             1392
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
14 -9 0 0.0389
-8 14 4 0.0346
-5 13 -9 0.0518
-13 9 -8 0.0532
-1 -4 29 0.1374
-7 14 -3 0.0334
-6 3 -28 0.1111
-2 -4 -29 0.119
-11 -2 -1 0.0361
-1 12 1 0.0351
-5 10 21 0.0984
2 -3 -31 0.1262
4 -2 30 0.1421
-3 3 31 0.1329
10 3 0 0.0426
-2 4 -30 0.1148
-10 -3 1 0.0394
1 11 1 0.0378
3 -13 -1 0.0369
-12 12 0 0.0295
-14 6 2 0.0338

_exptl_special_details           
;
 ?
;

#----------------------------------------------------------------------------#
#                   ABSORPTION CORRECTION                                    #
#----------------------------------------------------------------------------#

_exptl_absorpt_coefficient_mu    3.046
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   
;
        CrysAlisPro, Agilent Technologies,
        Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
        (compiled Aug 13 2014,18:06:01)
Analytical numeric absorption correction using a multifaceted crystal
                        model based on expressions derived by R.C. Clark & J.S.
        (Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
        Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_absorpt_correction_T_min  0.542
_exptl_absorpt_correction_T_max  0.842

#----------------------------------------------------------------------------#
#                   DATA COLLECTION                                          #
#----------------------------------------------------------------------------#

_diffrn_source                   'SuperNova (Mo) X-ray Source'
_diffrn_ambient_temperature      100(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_detector                 'CCD plate'
_diffrn_detector_type            Eos
_diffrn_detector_area_resol_mean 16.2439
_diffrn_orient_matrix_ub_11      0.0106359
_diffrn_orient_matrix_ub_12      -0.0414066
_diffrn_orient_matrix_ub_13      0.0238583
_diffrn_orient_matrix_ub_21      -0.0151703
_diffrn_orient_matrix_ub_22      0.0459929
_diffrn_orient_matrix_ub_23      0.0205945
_diffrn_orient_matrix_ub_31      -0.0820588
_diffrn_orient_matrix_ub_32      -0.0569794
_diffrn_orient_matrix_ub_33      -0.0007283
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'SuperNova, Single source at offset, Eos'
_diffrn_measurement_method       'ω scans'
_diffrn_reflns_av_R_equivalents  0.0383
_diffrn_reflns_av_unetI/netI     0.0233
_diffrn_reflns_number            13563
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_l_min       -29
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_theta_min         1.81
_diffrn_reflns_theta_max         28.34
_diffrn_measured_fraction_theta_max 0.953
_diffrn_reflns_theta_full        25.00
_diffrn_measured_fraction_theta_full 0.996
_reflns_number_total             1507
_reflns_number_gt                1431
_reflns_threshold_expression     >2sigma(I)

#----------------------------------------------------------------------------#
#                   COMPUTER PROGRAMS USED                                   #
#----------------------------------------------------------------------------#

_computing_data_collection       
;
        CrysAlisPro, Agilent Technologies,
        Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
        (compiled Aug 13 2014,18:06:01)
;
_computing_cell_refinement       
;
        CrysAlisPro, Agilent Technologies,
        Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
        (compiled Aug 13 2014,18:06:01)
;
_computing_data_reduction        
;
        CrysAlisPro, Agilent Technologies,
        Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
        (compiled Aug 13 2014,18:06:01)
;
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'

#----------------------------------------------------------------------------#
#                   STRUCTURE SOLUTION                                       #
#----------------------------------------------------------------------------#

_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom

#----------------------------------------------------------------------------#
#                   REFINEMENT INFORMATION                                   #
#----------------------------------------------------------------------------#

_refine_special_details          
;Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.,Twin
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0190P)²+1.4895P] where P=(Fo²+2Fc²)/3'
_refine_ls_hydrogen_treatment    mixed
_refine_ls_extinction_method     none
_refine_ls_number_reflns         1507
_refine_ls_number_parameters     108
_refine_ls_number_restraints     3
_refine_ls_R_factor_all          0.0259
_refine_ls_R_factor_gt           0.0241
_refine_ls_wR_factor_ref         0.054
_refine_ls_wR_factor_gt          0.0529
_refine_ls_goodness_of_fit_ref   1.053
_refine_ls_restrained_S_all      1.054
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0
_refine_diff_density_max         0.531
_refine_diff_density_min         -0.705
_refine_diff_density_rms         0.082

#----------------------------------------------------------------------------#
#                   CONSTRAINTS AND RESTRAINTS                               #
#----------------------------------------------------------------------------#


#----------------------------------------------------------------------------#
#                   ATOMIC TYPES, COORDINATES AND THERMAL PARAMETERS         #
#----------------------------------------------------------------------------#

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0 0 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.006 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mn1 Mn 0.31872(4) 0.33444(4) 0.877259(13) 0.00517(9) Uani 1 1 d . . .
K1 K 0.66975(6) 0.66080(6) 0.963989(19) 0.00892(11) Uani 1 1 d . . .
P1 P 0 0 0.91437(4) 0.0054(2) Uani 1 3 d S . .
P2 P 0.3333 0.6667 0.91715(4) 0.00484(18) Uani 1 3 d S . .
P3 P 0.6667 0.3333 0.89703(4) 0.00602(18) Uani 1 3 d S . .
O1 O 0.3437(2) 0.52105(19) 0.93607(7) 0.0075(3) Uani 1 1 d . . .
O2 O 0.15613(19) 0.14449(19) 0.93308(7) 0.0073(3) Uani 1 1 d . . .
O3 O 0.51748(18) 0.3353(2) 0.91663(7) 0.0094(3) Uani 1 1 d . . .
O4 O 0.4375(2) 0.4923(2) 0.79980(7) 0.0098(4) Uani 1 1 d . . .
O5W O 0.10264(18) 0.3341(2) 0.84221(7) 0.0110(3) Uani 1 1 d D . .
O6 O 0.2831(2) 0.17599(19) 0.79978(7) 0.0109(4) Uani 1 1 d . . .
C1 C 0.3149(5) 0.2423(4) 0.75 0.0080(7) Uani 1 2 d S . .
C2 C 0.4049(4) 0.4266(4) 0.75 0.0070(6) Uani 1 2 d S . .
H2 H 0.3333 0.6667 0.8578(18) 0.006(10) Uiso 1 3 d S . .
H3 H 0.6667 0.3333 0.8390(18) 0.015(11) Uiso 1 3 d S . .
H1 H 0 0 0.856(2) 0.018 Uiso 1 3 d S . .
H5A H 0.026(3) 0.258(2) 0.8262(12) 0.023(8) Uiso 1 1 d D . .
H5B H 0.108(3) 0.413(2) 0.8257(12) 0.023(9) Uiso 1 1 d D . .



#----------------------------------------------------------------------------#
#                   MOLECULAR GEOMETRY                                       #
#----------------------------------------------------------------------------#

_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mn1 O3 2.1246(14) . ?
Mn1 O2 2.1390(16) . ?
Mn1 O1 2.1608(15) . ?
Mn1 O4 2.2267(16) . ?
Mn1 O6 2.2367(16) . ?
Mn1 O5W 2.2454(14) . ?
Mn1 K1 3.5720(5) 7_667 ?
Mn1 K1 3.7225(5) 5_565 ?
Mn1 K1 3.8107(5) 3_655 ?
Mn1 K1 3.8373(6) . ?
K1 O2 2.785(2) 5_665 ?
K1 O1 2.8239(15) 7_667 ?
K1 O1 2.830(2) . ?
K1 O2 2.9351(17) 7_667 ?
K1 O5W 2.9401(17) 3_665 ?
K1 O3 2.946(2) . ?
K1 O3 2.9543(19) 5_665 ?
K1 O2 3.0407(19) 3_665 ?
K1 O1 3.042(2) 3_665 ?
K1 O3 3.2566(15) 7_667 ?
K1 P1 3.4459(6) 1_665 ?
K1 P2 3.4685(5) . ?
P1 O2 1.5260(15) 5 ?
P1 O2 1.5260(15) 3 ?
P1 O2 1.5260(16) . ?
P1 K1 3.4459(6) 1_445 ?
P1 K1 3.4459(6) 3_655 ?
P1 K1 3.4459(6) 5_565 ?
P1 H1 1.32(5) . ?
P2 O1 1.5311(15) 3_665 ?
P2 O1 1.5311(14) . ?
P2 O1 1.5311(14) 5_565 ?
P2 K1 3.4685(5) 3_665 ?
P2 K1 3.4685(5) 5_565 ?
P2 H2 1.33(4) . ?
P3 O3 1.5271(14) 3_655 ?
P3 O3 1.5271(14) 5_665 ?
P3 O3 1.5271(14) . ?
P3 K1 3.5129(6) 5_665 ?
P3 K1 3.5129(6) 3_655 ?
P3 H3 1.30(4) . ?
O1 K1 2.8239(15) 7_667 ?
O1 K1 3.042(2) 5_565 ?
O2 K1 2.7849(19) 3_655 ?
O2 K1 2.9351(16) 7_667 ?
O2 K1 3.0407(19) 5_565 ?
O3 K1 2.9543(19) 3_655 ?
O3 K1 3.2566(15) 7_667 ?
O4 C2 1.250(2) . ?
O5W K1 2.9401(17) 5_565 ?
O5W H5A 0.830(10) . ?
O5W H5B 0.827(10) . ?
O6 C1 1.252(2) . ?
C1 O6 1.252(2) 10_557 ?
C1 C2 1.554(4) . ?
C2 O4 1.250(2) 10_557 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O3 Mn1 O2 92.16(6) . . ?
O3 Mn1 O1 91.29(7) . . ?
O2 Mn1 O1 95.23(5) . . ?
O3 Mn1 O4 99.55(7) . . ?
O2 Mn1 O4 163.85(6) . . ?
O1 Mn1 O4 95.58(6) . . ?
O3 Mn1 O6 98.87(7) . . ?
O2 Mn1 O6 93.92(6) . . ?
O1 Mn1 O6 166.05(6) . . ?
O4 Mn1 O6 73.41(5) . . ?
O3 Mn1 O5W 175.92(6) . . ?
O2 Mn1 O5W 85.23(7) . . ?
O1 Mn1 O5W 85.84(7) . . ?
O4 Mn1 O5W 83.63(6) . . ?
O6 Mn1 O5W 84.45(6) . . ?
O3 Mn1 K1 63.94(4) . 7_667 ?
O2 Mn1 K1 55.21(4) . 7_667 ?
O1 Mn1 K1 52.23(4) . 7_667 ?
O4 Mn1 K1 140.45(5) . 7_667 ?
O6 Mn1 K1 141.34(4) . 7_667 ?
O5W Mn1 K1 111.98(4) . 7_667 ?
O3 Mn1 K1 123.76(4) . 5_565 ?
O2 Mn1 K1 54.77(5) . 5_565 ?
O1 Mn1 K1 54.81(6) . 5_565 ?
O4 Mn1 K1 124.33(5) . 5_565 ?
O6 Mn1 K1 124.35(5) . 5_565 ?
O5W Mn1 K1 52.16(4) . 5_565 ?
K1 Mn1 K1 59.834(10) 7_667 5_565 ?
O3 Mn1 K1 50.46(5) . 3_655 ?
O2 Mn1 K1 45.92(5) . 3_655 ?
O1 Mn1 K1 110.82(4) . 3_655 ?
O4 Mn1 K1 138.56(5) . 3_655 ?
O6 Mn1 K1 83.09(4) . 3_655 ?
O5W Mn1 K1 128.11(5) . 3_655 ?
K1 Mn1 K1 58.983(10) 7_667 3_655 ?
K1 Mn1 K1 97.101(16) 5_565 3_655 ?
O3 Mn1 K1 49.65(5) . . ?
O2 Mn1 K1 112.67(4) . . ?
O1 Mn1 K1 46.63(5) . . ?
O4 Mn1 K1 83.45(5) . . ?
O6 Mn1 K1 137.23(5) . . ?
O5W Mn1 K1 128.74(5) . . ?
K1 Mn1 K1 58.120(14) 7_667 . ?
K1 Mn1 K1 98.414(15) 5_565 . ?
K1 Mn1 K1 91.900(15) 3_655 . ?
O2 K1 O1 106.71(5) 5_665 7_667 ?
O2 K1 O1 151.10(4) 5_665 . ?
O1 K1 O1 100.73(5) 7_667 . ?
O2 K1 O2 71.62(7) 5_665 7_667 ?
O1 K1 O2 66.91(4) 7_667 7_667 ?
O1 K1 O2 129.24(5) . 7_667 ?
O2 K1 O5W 75.40(5) 5_665 3_665 ?
O1 K1 O5W 163.85(4) 7_667 3_665 ?
O1 K1 O5W 75.72(5) . 3_665 ?
O2 K1 O5W 127.64(5) 7_667 3_665 ?
O2 K1 O3 113.49(5) 5_665 . ?
O1 K1 O3 76.86(5) 7_667 . ?
O1 K1 O3 64.04(4) . . ?
O2 K1 O3 142.90(5) 7_667 . ?
O5W K1 O3 87.58(4) 3_665 . ?
O2 K1 O3 64.62(4) 5_665 5_665 ?
O1 K1 O3 78.57(5) 7_667 5_665 ?
O1 K1 O3 113.40(4) . 5_665 ?
O2 K1 O3 111.72(5) 7_667 5_665 ?
O5W K1 O3 88.32(4) 3_665 5_665 ?
O3 K1 O3 50.83(5) . 5_665 ?
O2 K1 O2 51.48(6) 5_665 3_665 ?
O1 K1 O2 134.55(6) 7_667 3_665 ?
O1 K1 O2 112.56(5) . 3_665 ?
O2 K1 O2 68.14(6) 7_667 3_665 ?
O5W K1 O2 59.51(5) 3_665 3_665 ?
O3 K1 O2 145.35(5) . 3_665 ?
O3 K1 O2 112.75(4) 5_665 3_665 ?
O2 K1 O1 112.97(5) 5_665 3_665 ?
O1 K1 O1 129.82(4) 7_667 3_665 ?
O1 K1 O1 51.27(5) . 3_665 ?
O2 K1 O1 97.67(5) 7_667 3_665 ?
O5W K1 O1 60.19(4) 3_665 3_665 ?
O3 K1 O1 111.93(4) . 3_665 ?
O3 K1 O1 146.47(5) 5_665 3_665 ?
O2 K1 O1 62.95(4) 3_665 3_665 ?
O2 K1 O3 130.49(5) 5_665 7_667 ?
O1 K1 O3 60.02(4) 7_667 7_667 ?
O1 K1 O3 71.85(4) . 7_667 ?
O2 K1 O3 59.20(4) 7_667 7_667 ?
O5W K1 O3 131.06(4) 3_665 7_667 ?
O3 K1 O3 109.10(4) . 7_667 ?
O3 K1 O3 138.13(4) 5_665 7_667 ?
O2 K1 O3 101.38(5) 3_665 7_667 ?
O1 K1 O3 70.96(4) 3_665 7_667 ?
O2 K1 P1 25.65(3) 5_665 1_665 ?
O1 K1 P1 125.96(5) 7_667 1_665 ?
O1 K1 P1 132.38(3) . 1_665 ?
O2 K1 P1 71.07(4) 7_667 1_665 ?
O5W K1 P1 61.87(4) 3_665 1_665 ?
O3 K1 P1 129.83(3) . 1_665 ?
O3 K1 P1 87.18(3) 5_665 1_665 ?
O2 K1 P1 26.27(3) 3_665 1_665 ?
O1 K1 P1 87.45(3) 3_665 1_665 ?
O3 K1 P1 121.02(4) 7_667 1_665 ?
O2 K1 P2 132.27(4) 5_665 . ?
O1 K1 P2 120.28(5) 7_667 . ?
O1 K1 P2 25.66(3) . . ?
O2 K1 P2 118.31(4) 7_667 . ?
O5W K1 P2 62.00(4) 3_665 . ?
O3 K1 P2 86.36(3) . . ?
O3 K1 P2 129.97(4) 5_665 . ?
O2 K1 P2 87.03(3) 3_665 . ?
O1 K1 P2 26.16(3) 3_665 . ?
O3 K1 P2 73.23(3) 7_667 . ?
P1 K1 P2 108.798(15) 1_665 . ?
O2 P1 O2 112.71(6) 5 3 ?
O2 P1 O2 112.71(6) 5 . ?
O2 P1 O2 112.70(6) 3 . ?
O2 P1 K1 52.19(7) 5 1_445 ?
O2 P1 K1 61.88(7) 3 1_445 ?
O2 P1 K1 144.73(8) . 1_445 ?
O2 P1 K1 61.88(7) 5 3_655 ?
O2 P1 K1 144.73(8) 3 3_655 ?
O2 P1 K1 52.19(7) . 3_655 ?
K1 P1 K1 110.039(15) 1_445 3_655 ?
O2 P1 K1 144.73(8) 5 5_565 ?
O2 P1 K1 52.19(7) 3 5_565 ?
O2 P1 K1 61.88(7) . 5_565 ?
K1 P1 K1 110.039(15) 1_445 5_565 ?
K1 P1 K1 110.039(15) 3_655 5_565 ?
O2 P1 H1 106.00(7) 5 . ?
O2 P1 H1 106.00(7) 3 . ?
O2 P1 H1 106.00(7) . . ?
K1 P1 H1 108.90(2) 1_445 . ?
K1 P1 H1 108.897(18) 3_655 . ?
K1 P1 H1 108.897(17) 5_565 . ?
O1 P2 O1 112.59(6) 3_665 . ?
O1 P2 O1 112.59(6) 3_665 5_565 ?
O1 P2 O1 112.59(6) . 5_565 ?
O1 P2 K1 53.16(8) 3_665 3_665 ?
O1 P2 K1 145.92(7) . 3_665 ?
O1 P2 K1 61.18(8) 5_565 3_665 ?
O1 P2 K1 145.93(7) 3_665 5_565 ?
O1 P2 K1 61.19(8) . 5_565 ?
O1 P2 K1 53.16(8) 5_565 5_565 ?
K1 P2 K1 111.200(14) 3_665 5_565 ?
O1 P2 K1 61.19(8) 3_665 . ?
O1 P2 K1 53.16(8) . . ?
O1 P2 K1 145.93(7) 5_565 . ?
K1 P2 K1 111.200(14) 3_665 . ?
K1 P2 K1 111.200(14) 5_565 . ?
O1 P2 H2 106.13(7) 3_665 . ?
O1 P2 H2 106.14(6) . . ?
O1 P2 H2 106.13(6) 5_565 . ?
K1 P2 H2 107.682(16) 3_665 . ?
K1 P2 H2 107.68(2) 5_565 . ?
K1 P2 H2 107.682(17) . . ?
O3 P3 O3 112.03(6) 3_655 5_665 ?
O3 P3 O3 112.03(6) 3_655 . ?
O3 P3 O3 112.03(6) 5_665 . ?
O3 P3 K1 56.35(7) 3_655 5_665 ?
O3 P3 K1 56.05(7) 5_665 5_665 ?
O3 P3 K1 137.83(7) . 5_665 ?
O3 P3 K1 56.05(7) 3_655 3_655 ?
O3 P3 K1 137.83(7) 5_665 3_655 ?
O3 P3 K1 56.35(7) . 3_655 ?
K1 P3 K1 102.960(18) 5_665 3_655 ?
O3 P3 K1 137.83(7) 3_655 . ?
O3 P3 K1 56.35(7) 5_665 . ?
O3 P3 K1 56.05(8) . . ?
K1 P3 K1 102.960(18) 5_665 . ?
K1 P3 K1 102.960(18) 3_655 . ?
O3 P3 H3 106.78(7) 3_655 . ?
O3 P3 H3 106.78(7) 5_665 . ?
O3 P3 H3 106.78(7) . . ?
K1 P3 H3 115.388(17) 5_665 . ?
K1 P3 H3 115.39(2) 3_655 . ?
K1 P3 H3 115.388(16) . . ?
P2 O1 Mn1 125.23(9) . . ?
P2 O1 K1 142.95(9) . 7_667 ?
Mn1 O1 K1 90.54(5) . 7_667 ?
P2 O1 K1 101.18(9) . . ?
Mn1 O1 K1 99.64(6) . . ?
K1 O1 K1 79.27(5) 7_667 . ?
P2 O1 K1 92.65(8) . 5_565 ?
Mn1 O1 K1 89.70(6) . 5_565 ?
K1 O1 K1 76.62(5) 7_667 5_565 ?
K1 O1 K1 154.19(6) . 5_565 ?
P1 O2 Mn1 126.93(10) . . ?
P1 O2 K1 102.15(8) . 3_655 ?
Mn1 O2 K1 100.60(6) . 3_655 ?
P1 O2 K1 143.17(9) . 7_667 ?
Mn1 O2 K1 88.03(5) . 7_667 ?
K1 O2 K1 79.01(4) 3_655 7_667 ?
P1 O2 K1 91.85(8) . 5_565 ?
Mn1 O2 K1 90.16(6) . 5_565 ?
K1 O2 K1 151.50(6) 3_655 5_565 ?
K1 O2 K1 75.04(4) 7_667 5_565 ?
P3 O3 Mn1 138.58(10) . . ?
P3 O3 K1 98.48(8) . . ?
Mn1 O3 K1 97.02(6) . . ?
P3 O3 K1 98.16(8) . 3_655 ?
Mn1 O3 K1 95.85(6) . 3_655 ?
K1 O3 K1 137.36(6) . 3_655 ?
P3 O3 K1 141.23(8) . 7_667 ?
Mn1 O3 K1 80.18(4) . 7_667 ?
K1 O3 K1 70.90(4) . 7_667 ?
K1 O3 K1 71.58(4) 3_655 7_667 ?
C2 O4 Mn1 115.88(17) . . ?
Mn1 O5W K1 90.74(5) . 5_565 ?
Mn1 O5W H5A 126(2) . . ?
K1 O5W H5A 103(2) 5_565 . ?
Mn1 O5W H5B 122(2) . . ?
K1 O5W H5B 107(2) 5_565 . ?
H5A O5W H5B 104.2(19) . . ?
C1 O6 Mn1 115.34(17) . . ?
O6 C1 O6 126.9(3) 10_557 . ?
O6 C1 C2 116.55(16) 10_557 . ?
O6 C1 C2 116.55(16) . . ?
O4 C2 O4 127.3(3) 10_557 . ?
O4 C2 C1 116.32(16) 10_557 . ?
O4 C2 C1 116.32(16) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 K1 P2 O1 -49.15(10) 5_665 . . 3_665 ?
O1 K1 P2 O1 119.55(5) 7_667 . . 3_665 ?
O1 K1 P2 O1 163.72(14) . . . 3_665 ?
O2 K1 P2 O1 41.17(8) 7_667 . . 3_665 ?
O5W K1 P2 O1 -78.78(8) 3_665 . . 3_665 ?
O3 K1 P2 O1 -167.96(8) . . . 3_665 ?
O3 K1 P2 O1 -139.50(8) 5_665 . . 3_665 ?
O2 K1 P2 O1 -21.99(8) 3_665 . . 3_665 ?
O3 K1 P2 O1 80.83(8) 7_667 . . 3_665 ?
P1 K1 P2 O1 -36.94(7) 1_665 . . 3_665 ?
O2 K1 P2 O1 147.14(8) 5_665 . . . ?
O1 K1 P2 O1 -44.17(10) 7_667 . . . ?
O2 K1 P2 O1 -122.55(9) 7_667 . . . ?
O5W K1 P2 O1 117.50(9) 3_665 . . . ?
O3 K1 P2 O1 28.32(8) . . . . ?
O3 K1 P2 O1 56.78(9) 5_665 . . . ?
O2 K1 P2 O1 174.29(8) 3_665 . . . ?
O1 K1 P2 O1 -163.72(14) 3_665 . . . ?
O3 K1 P2 O1 -82.89(9) 7_667 . . . ?
P1 K1 P2 O1 159.34(8) 1_665 . . . ?
O2 K1 P2 O1 -137.39(14) 5_665 . . 5_565 ?
O1 K1 P2 O1 31.31(13) 7_667 . . 5_565 ?
O1 K1 P2 O1 75.48(13) . . . 5_565 ?
O2 K1 P2 O1 -47.07(14) 7_667 . . 5_565 ?
O5W K1 P2 O1 -167.02(14) 3_665 . . 5_565 ?
O3 K1 P2 O1 103.80(14) . . . 5_565 ?
O3 K1 P2 O1 132.26(14) 5_665 . . 5_565 ?
O2 K1 P2 O1 -110.24(14) 3_665 . . 5_565 ?
O1 K1 P2 O1 -88.24(14) 3_665 . . 5_565 ?
O3 K1 P2 O1 -7.41(15) 7_667 . . 5_565 ?
P1 K1 P2 O1 -125.18(14) 1_665 . . 5_565 ?
O2 K1 P2 K1 -67.83(6) 5_665 . . 3_665 ?
O1 K1 P2 K1 100.87(4) 7_667 . . 3_665 ?
O1 K1 P2 K1 145.03(8) . . . 3_665 ?
O2 K1 P2 K1 22.49(5) 7_667 . . 3_665 ?
O5W K1 P2 K1 -97.46(4) 3_665 . . 3_665 ?
O3 K1 P2 K1 173.35(4) . . . 3_665 ?
O3 K1 P2 K1 -158.19(4) 5_665 . . 3_665 ?
O2 K1 P2 K1 -40.68(4) 3_665 . . 3_665 ?
O1 K1 P2 K1 -18.69(7) 3_665 . . 3_665 ?
O3 K1 P2 K1 62.15(4) 7_667 . . 3_665 ?
P1 K1 P2 K1 -55.63(3) 1_665 . . 3_665 ?
O2 K1 P2 K1 167.66(5) 5_665 . . 5_565 ?
O1 K1 P2 K1 -23.64(5) 7_667 . . 5_565 ?
O1 K1 P2 K1 20.53(7) . . . 5_565 ?
O2 K1 P2 K1 -102.02(4) 7_667 . . 5_565 ?
O5W K1 P2 K1 138.03(4) 3_665 . . 5_565 ?
O3 K1 P2 K1 48.85(4) . . . 5_565 ?
O3 K1 P2 K1 77.31(5) 5_665 . . 5_565 ?
O2 K1 P2 K1 -165.18(4) 3_665 . . 5_565 ?
O1 K1 P2 K1 -143.19(8) 3_665 . . 5_565 ?
O3 K1 P2 K1 -62.36(4) 7_667 . . 5_565 ?
P1 K1 P2 K1 179.87(2) 1_665 . . 5_565 ?
O2 K1 P3 O3 105.58(12) 5_665 . . 3_655 ?
O1 K1 P3 O3 -1.82(13) 7_667 . . 3_655 ?
O1 K1 P3 O3 -103.15(12) . . . 3_655 ?
O2 K1 P3 O3 41.96(12) 7_667 . . 3_655 ?
O5W K1 P3 O3 -178.96(12) 3_665 . . 3_655 ?
O3 K1 P3 O3 -85.99(11) . . . 3_655 ?
O3 K1 P3 O3 86.34(11) 5_665 . . 3_655 ?
O2 K1 P3 O3 138.13(12) 3_665 . . 3_655 ?
O1 K1 P3 O3 -134.87(12) 3_665 . . 3_655 ?
O3 K1 P3 O3 -37.85(11) 7_667 . . 3_655 ?
P1 K1 P3 O3 122.44(11) 1_665 . . 3_655 ?
P2 K1 P3 O3 -120.10(11) . . . 3_655 ?
O2 K1 P3 O3 19.24(8) 5_665 . . 5_665 ?
O1 K1 P3 O3 -88.16(9) 7_667 . . 5_665 ?
O1 K1 P3 O3 170.51(9) . . . 5_665 ?
O2 K1 P3 O3 -44.38(9) 7_667 . . 5_665 ?
O5W K1 P3 O3 94.70(9) 3_665 . . 5_665 ?
O3 K1 P3 O3 -172.34(14) . . . 5_665 ?
O2 K1 P3 O3 51.79(9) 3_665 . . 5_665 ?
O1 K1 P3 O3 138.79(9) 3_665 . . 5_665 ?
O3 K1 P3 O3 -124.19(6) 7_667 . . 5_665 ?
P1 K1 P3 O3 36.09(8) 1_665 . . 5_665 ?
P2 K1 P3 O3 153.56(8) . . . 5_665 ?
O2 K1 P3 O3 -168.42(9) 5_665 . . . ?
O1 K1 P3 O3 84.18(9) 7_667 . . . ?
O1 K1 P3 O3 -17.16(8) . . . . ?
O2 K1 P3 O3 127.95(9) 7_667 . . . ?
O5W K1 P3 O3 -92.96(8) 3_665 . . . ?
O3 K1 P3 O3 172.34(14) 5_665 . . . ?
O2 K1 P3 O3 -135.87(8) 3_665 . . . ?
O1 K1 P3 O3 -48.87(9) 3_665 . . . ?
O3 K1 P3 O3 48.14(10) 7_667 . . . ?
P1 K1 P3 O3 -151.57(8) 1_665 . . . ?
P2 K1 P3 O3 -34.11(8) . . . . ?
O2 K1 P3 K1 51.94(4) 5_665 . . 5_665 ?
O1 K1 P3 K1 -55.46(5) 7_667 . . 5_665 ?
O1 K1 P3 K1 -156.79(3) . . . 5_665 ?
O2 K1 P3 K1 -11.68(5) 7_667 . . 5_665 ?
O5W K1 P3 K1 127.40(4) 3_665 . . 5_665 ?
O3 K1 P3 K1 -139.64(8) . . . 5_665 ?
O3 K1 P3 K1 32.70(7) 5_665 . . 5_665 ?
O2 K1 P3 K1 84.49(5) 3_665 . . 5_665 ?
O1 K1 P3 K1 171.49(4) 3_665 . . 5_665 ?
O3 K1 P3 K1 -91.49(3) 7_667 . . 5_665 ?
P1 K1 P3 K1 68.80(3) 1_665 . . 5_665 ?
P2 K1 P3 K1 -173.743(17) . . . 5_665 ?
O2 K1 P3 K1 158.75(4) 5_665 . . 3_655 ?
O1 K1 P3 K1 51.35(5) 7_667 . . 3_655 ?
O1 K1 P3 K1 -49.99(4) . . . 3_655 ?
O2 K1 P3 K1 95.12(4) 7_667 . . 3_655 ?
O5W K1 P3 K1 -125.79(4) 3_665 . . 3_655 ?
O3 K1 P3 K1 -32.83(7) . . . 3_655 ?
O3 K1 P3 K1 139.51(8) 5_665 . . 3_655 ?
O2 K1 P3 K1 -168.70(4) 3_665 . . 3_655 ?
O1 K1 P3 K1 -81.71(5) 3_665 . . 3_655 ?
O3 K1 P3 K1 15.31(4) 7_667 . . 3_655 ?
P1 K1 P3 K1 175.600(18) 1_665 . . 3_655 ?
P2 K1 P3 K1 -66.94(3) . . . 3_655 ?
O1 P2 O1 Mn1 -125.83(16) 3_665 . . . ?
O1 P2 O1 Mn1 105.58(17) 5_565 . . . ?
K1 P2 O1 Mn1 177.12(2) 3_665 . . . ?
K1 P2 O1 Mn1 91.51(13) 5_565 . . . ?
K1 P2 O1 Mn1 -110.40(14) . . . . ?
O1 P2 O1 K1 71.52(16) 3_665 . . 7_667 ?
O1 P2 O1 K1 -57.08(18) 5_565 . . 7_667 ?
K1 P2 O1 K1 14.5(3) 3_665 . . 7_667 ?
K1 P2 O1 K1 -71.14(16) 5_565 . . 7_667 ?
K1 P2 O1 K1 86.95(17) . . . 7_667 ?
O1 P2 O1 K1 -15.43(13) 3_665 . . . ?
O1 P2 O1 K1 -144.03(5) 5_565 . . . ?
K1 P2 O1 K1 -72.48(13) 3_665 . . . ?
K1 P2 O1 K1 -158.09(7) 5_565 . . . ?
O1 P2 O1 K1 142.66(6) 3_665 . . 5_565 ?
O1 P2 O1 K1 14.06(12) 5_565 . . 5_565 ?
K1 P2 O1 K1 85.61(12) 3_665 . . 5_565 ?
K1 P2 O1 K1 158.09(7) . . . 5_565 ?
O3 Mn1 O1 P2 135.33(15) . . . . ?
O2 Mn1 O1 P2 -132.38(15) . . . . ?
O4 Mn1 O1 P2 35.61(14) . . . . ?
O6 Mn1 O1 P2 -1.6(4) . . . . ?
O5W Mn1 O1 P2 -47.56(14) . . . . ?
K1 Mn1 O1 P2 -169.65(17) 7_667 . . . ?
K1 Mn1 O1 P2 -93.04(14) 5_565 . . . ?
K1 Mn1 O1 P2 -176.94(11) 3_655 . . . ?
K1 Mn1 O1 P2 111.14(15) . . . . ?
O3 Mn1 O1 K1 -55.02(6) . . . 7_667 ?
O2 Mn1 O1 K1 37.27(5) . . . 7_667 ?
O4 Mn1 O1 K1 -154.74(6) . . . 7_667 ?
O6 Mn1 O1 K1 168.1(3) . . . 7_667 ?
O5W Mn1 O1 K1 122.09(6) . . . 7_667 ?
K1 Mn1 O1 K1 76.61(5) 5_565 . . 7_667 ?
K1 Mn1 O1 K1 -7.29(6) 3_655 . . 7_667 ?
K1 Mn1 O1 K1 -79.21(5) . . . 7_667 ?
O3 Mn1 O1 K1 24.19(6) . . . . ?
O2 Mn1 O1 K1 116.48(6) . . . . ?
O4 Mn1 O1 K1 -75.54(6) . . . . ?
O6 Mn1 O1 K1 -112.7(3) . . . . ?
O5W Mn1 O1 K1 -158.71(6) . . . . ?
K1 Mn1 O1 K1 79.21(5) 7_667 . . . ?
K1 Mn1 O1 K1 155.82(6) 5_565 . . . ?
K1 Mn1 O1 K1 71.92(5) 3_655 . . . ?
O3 Mn1 O1 K1 -131.63(5) . . . 5_565 ?
O2 Mn1 O1 K1 -39.34(5) . . . 5_565 ?
O4 Mn1 O1 K1 128.64(5) . . . 5_565 ?
O6 Mn1 O1 K1 91.5(3) . . . 5_565 ?
O5W Mn1 O1 K1 45.47(5) . . . 5_565 ?
K1 Mn1 O1 K1 -76.61(5) 7_667 . . 5_565 ?
K1 Mn1 O1 K1 -83.90(4) 3_655 . . 5_565 ?
K1 Mn1 O1 K1 -155.82(6) . . . 5_565 ?
O2 K1 O1 P2 -56.19(12) 5_665 . . . ?
O1 K1 O1 P2 142.23(9) 7_667 . . . ?
O2 K1 O1 P2 73.38(9) 7_667 . . . ?
O5W K1 O1 P2 -53.91(7) 3_665 . . . ?
O3 K1 O1 P2 -148.23(9) . . . . ?
O3 K1 O1 P2 -135.69(7) 5_665 . . . ?
O2 K1 O1 P2 -6.18(9) 3_665 . . . ?
O1 K1 O1 P2 9.12(8) 3_665 . . . ?
O3 K1 O1 P2 88.91(8) 7_667 . . . ?
P1 K1 O1 P2 -26.88(10) 1_665 . . . ?
O2 K1 O1 Mn1 72.86(10) 5_665 . . . ?
O1 K1 O1 Mn1 -88.72(5) 7_667 . . . ?
O2 K1 O1 Mn1 -157.58(6) 7_667 . . . ?
O5W K1 O1 Mn1 75.14(5) 3_665 . . . ?
O3 K1 O1 Mn1 -19.18(5) . . . . ?
O3 K1 O1 Mn1 -6.64(7) 5_665 . . . ?
O2 K1 O1 Mn1 122.87(6) 3_665 . . . ?
O1 K1 O1 Mn1 138.17(5) 3_665 . . . ?
O3 K1 O1 Mn1 -142.04(6) 7_667 . . . ?
P1 K1 O1 Mn1 102.16(5) 1_665 . . . ?
P2 K1 O1 Mn1 129.05(11) . . . . ?
O2 K1 O1 K1 161.58(8) 5_665 . . 7_667 ?
O1 K1 O1 K1 0 7_667 . . 7_667 ?
O2 K1 O1 K1 -68.86(6) 7_667 . . 7_667 ?
O5W K1 O1 K1 163.85(4) 3_665 . . 7_667 ?
O3 K1 O1 K1 69.54(4) . . . 7_667 ?
O3 K1 O1 K1 82.08(5) 5_665 . . 7_667 ?
O2 K1 O1 K1 -148.41(4) 3_665 . . 7_667 ?
O1 K1 O1 K1 -133.12(3) 3_665 . . 7_667 ?
O3 K1 O1 K1 -53.33(4) 7_667 . . 7_667 ?
P1 K1 O1 K1 -169.12(3) 1_665 . . 7_667 ?
P2 K1 O1 K1 -142.23(9) . . . 7_667 ?
O2 K1 O1 K1 -177.30(11) 5_665 . . 5_565 ?
O1 K1 O1 K1 21.12(10) 7_667 . . 5_565 ?
O2 K1 O1 K1 -47.74(14) 7_667 . . 5_565 ?
O5W K1 O1 K1 -175.03(13) 3_665 . . 5_565 ?
O3 K1 O1 K1 90.66(13) . . . 5_565 ?
O3 K1 O1 K1 103.20(13) 5_665 . . 5_565 ?
O2 K1 O1 K1 -127.29(12) 3_665 . . 5_565 ?
O1 K1 O1 K1 -112.00(12) 3_665 . . 5_565 ?
O3 K1 O1 K1 -32.21(12) 7_667 . . 5_565 ?
P1 K1 O1 K1 -148.00(10) 1_665 . . 5_565 ?
P2 K1 O1 K1 -121.11(17) . . . 5_565 ?
O2 P1 O2 Mn1 127.16(15) 5 . . . ?
O2 P1 O2 Mn1 -103.89(18) 3 . . . ?
K1 P1 O2 Mn1 -176.84(2) 1_445 . . . ?
K1 P1 O2 Mn1 113.40(14) 3_655 . . . ?
K1 P1 O2 Mn1 -91.59(12) 5_565 . . . ?
O2 P1 O2 K1 13.76(14) 5 . . 3_655 ?
O2 P1 O2 K1 142.71(5) 3 . . 3_655 ?
K1 P1 O2 K1 69.76(13) 1_445 . . 3_655 ?
K1 P1 O2 K1 155.01(8) 5_565 . . 3_655 ?
O2 P1 O2 K1 -74.07(15) 5 . . 7_667 ?
O2 P1 O2 K1 54.88(18) 3 . . 7_667 ?
K1 P1 O2 K1 -18.1(2) 1_445 . . 7_667 ?
K1 P1 O2 K1 -87.83(16) 3_655 . . 7_667 ?
K1 P1 O2 K1 67.18(14) 5_565 . . 7_667 ?
O2 P1 O2 K1 -141.25(7) 5 . . 5_565 ?
O2 P1 O2 K1 -12.30(12) 3 . . 5_565 ?
K1 P1 O2 K1 -85.25(11) 1_445 . . 5_565 ?
K1 P1 O2 K1 -155.01(8) 3_655 . . 5_565 ?
O3 Mn1 O2 P1 -136.71(14) . . . . ?
O1 Mn1 O2 P1 131.80(14) . . . . ?
O4 Mn1 O2 P1 -0.1(4) . . . . ?
O6 Mn1 O2 P1 -37.66(13) . . . . ?
O5W Mn1 O2 P1 46.43(13) . . . . ?
K1 Mn1 O2 P1 167.46(16) 7_667 . . . ?
K1 Mn1 O2 P1 92.43(13) 5_565 . . . ?
K1 Mn1 O2 P1 -114.12(15) 3_655 . . . ?
K1 Mn1 O2 P1 176.64(10) . . . . ?
O3 Mn1 O2 K1 -22.59(6) . . . 3_655 ?
O1 Mn1 O2 K1 -114.09(6) . . . 3_655 ?
O4 Mn1 O2 K1 114.1(2) . . . 3_655 ?
O6 Mn1 O2 K1 76.46(6) . . . 3_655 ?
O5W Mn1 O2 K1 160.55(6) . . . 3_655 ?
K1 Mn1 O2 K1 -78.43(5) 7_667 . . 3_655 ?
K1 Mn1 O2 K1 -153.45(7) 5_565 . . 3_655 ?
K1 Mn1 O2 K1 -69.24(6) . . . 3_655 ?
O3 Mn1 O2 K1 55.84(5) . . . 7_667 ?
O1 Mn1 O2 K1 -35.66(5) . . . 7_667 ?
O4 Mn1 O2 K1 -167.5(2) . . . 7_667 ?
O6 Mn1 O2 K1 154.89(6) . . . 7_667 ?
O5W Mn1 O2 K1 -121.02(6) . . . 7_667 ?
K1 Mn1 O2 K1 -75.02(4) 5_565 . . 7_667 ?
K1 Mn1 O2 K1 78.43(5) 3_655 . . 7_667 ?
K1 Mn1 O2 K1 9.19(6) . . . 7_667 ?
O3 Mn1 O2 K1 130.86(5) . . . 5_565 ?
O1 Mn1 O2 K1 39.37(5) . . . 5_565 ?
O4 Mn1 O2 K1 -92.5(3) . . . 5_565 ?
O6 Mn1 O2 K1 -130.09(5) . . . 5_565 ?
O5W Mn1 O2 K1 -46.00(5) . . . 5_565 ?
K1 Mn1 O2 K1 75.02(4) 7_667 . . 5_565 ?
K1 Mn1 O2 K1 153.45(7) 3_655 . . 5_565 ?
K1 Mn1 O2 K1 84.21(4) . . . 5_565 ?
O3 P3 O3 Mn1 -115.4(2) 3_655 . . . ?
O3 P3 O3 Mn1 117.7(2) 5_665 . . . ?
K1 P3 O3 Mn1 -179.07(9) 5_665 . . . ?
K1 P3 O3 Mn1 -108.55(19) 3_655 . . . ?
K1 P3 O3 Mn1 110.84(19) . . . . ?
O3 P3 O3 K1 133.75(6) 3_655 . . . ?
O3 P3 O3 K1 6.88(12) 5_665 . . . ?
K1 P3 O3 K1 70.09(11) 5_665 . . . ?
K1 P3 O3 K1 140.60(7) 3_655 . . . ?
O3 P3 O3 K1 -6.85(12) 3_655 . . 3_655 ?
O3 P3 O3 K1 -133.73(6) 5_665 . . 3_655 ?
K1 P3 O3 K1 -70.52(11) 5_665 . . 3_655 ?
K1 P3 O3 K1 -140.60(7) . . . 3_655 ?
O3 P3 O3 K1 63.80(16) 3_655 . . 7_667 ?
O3 P3 O3 K1 -63.08(15) 5_665 . . 7_667 ?
K1 P3 O3 K1 0.1(2) 5_665 . . 7_667 ?
K1 P3 O3 K1 70.65(14) 3_655 . . 7_667 ?
K1 P3 O3 K1 -69.96(14) . . . 7_667 ?
O2 Mn1 O3 P3 130.34(19) . . . . ?
O1 Mn1 O3 P3 -134.37(19) . . . . ?
O4 Mn1 O3 P3 -38.50(19) . . . . ?
O6 Mn1 O3 P3 36.03(19) . . . . ?
O5W Mn1 O3 P3 -18E1(6) . . . . ?
K1 Mn1 O3 P3 179.5(2) 7_667 . . . ?
K1 Mn1 O3 P3 178.34(14) 5_565 . . . ?
K1 Mn1 O3 P3 109.38(19) 3_655 . . . ?
K1 Mn1 O3 P3 -111.36(19) . . . . ?
O2 Mn1 O3 K1 -118.30(6) . . . . ?
O1 Mn1 O3 K1 -23.01(6) . . . . ?
O4 Mn1 O3 K1 72.86(6) . . . . ?
O6 Mn1 O3 K1 147.39(5) . . . . ?
O5W Mn1 O3 K1 -68.2(11) . . . . ?
K1 Mn1 O3 K1 -69.15(4) 7_667 . . . ?
K1 Mn1 O3 K1 -70.30(6) 5_565 . . . ?
K1 Mn1 O3 K1 -139.26(7) 3_655 . . . ?
O2 Mn1 O3 K1 20.97(6) . . . 3_655 ?
O1 Mn1 O3 K1 116.25(6) . . . 3_655 ?
O4 Mn1 O3 K1 -147.87(5) . . . 3_655 ?
O6 Mn1 O3 K1 -73.35(6) . . . 3_655 ?
O5W Mn1 O3 K1 71.1(11) . . . 3_655 ?
K1 Mn1 O3 K1 70.12(4) 7_667 . . 3_655 ?
K1 Mn1 O3 K1 68.96(6) 5_565 . . 3_655 ?
K1 Mn1 O3 K1 139.26(7) . . . 3_655 ?
O2 Mn1 O3 K1 -49.15(5) . . . 7_667 ?
O1 Mn1 O3 K1 46.14(5) . . . 7_667 ?
O4 Mn1 O3 K1 142.01(5) . . . 7_667 ?
O6 Mn1 O3 K1 -143.46(5) . . . 7_667 ?
O5W Mn1 O3 K1 1.0(11) . . . 7_667 ?
K1 Mn1 O3 K1 -1.15(6) 5_565 . . 7_667 ?
K1 Mn1 O3 K1 -70.12(4) 3_655 . . 7_667 ?
K1 Mn1 O3 K1 69.15(4) . . . 7_667 ?
O2 K1 O3 P3 12.64(9) 5_665 . . . ?
O1 K1 O3 P3 -90.10(8) 7_667 . . . ?
O1 K1 O3 P3 160.86(9) . . . . ?
O2 K1 O3 P3 -77.63(10) 7_667 . . . ?
O5W K1 O3 P3 85.57(8) 3_665 . . . ?
O3 K1 O3 P3 -4.24(8) 5_665 . . . ?
O2 K1 O3 P3 68.21(10) 3_665 . . . ?
O1 K1 O3 P3 141.96(7) 3_665 . . . ?
O3 K1 O3 P3 -141.50(8) 7_667 . . . ?
P1 K1 O3 P3 36.10(9) 1_665 . . . ?
P2 K1 O3 P3 147.65(7) . . . . ?
O2 K1 O3 Mn1 -128.83(5) 5_665 . . . ?
O1 K1 O3 Mn1 128.43(6) 7_667 . . . ?
O1 K1 O3 Mn1 19.39(5) . . . . ?
O2 K1 O3 Mn1 140.90(7) 7_667 . . . ?
O5W K1 O3 Mn1 -55.91(6) 3_665 . . . ?
O3 K1 O3 Mn1 -145.72(6) 5_665 . . . ?
O2 K1 O3 Mn1 -73.26(8) 3_665 . . . ?
O1 K1 O3 Mn1 0.49(7) 3_665 . . . ?
O3 K1 O3 Mn1 77.03(5) 7_667 . . . ?
P1 K1 O3 Mn1 -105.38(5) 1_665 . . . ?
P2 K1 O3 Mn1 6.18(5) . . . . ?
O2 K1 O3 K1 124.59(7) 5_665 . . 3_655 ?
O1 K1 O3 K1 21.85(7) 7_667 . . 3_655 ?
O1 K1 O3 K1 -87.19(8) . . . 3_655 ?
O2 K1 O3 K1 34.32(11) 7_667 . . 3_655 ?
O5W K1 O3 K1 -162.49(8) 3_665 . . 3_655 ?
O3 K1 O3 K1 107.70(7) 5_665 . . 3_655 ?
O2 K1 O3 K1 -179.84(7) 3_665 . . 3_655 ?
O1 K1 O3 K1 -106.09(8) 3_665 . . 3_655 ?
O3 K1 O3 K1 -29.55(6) 7_667 . . 3_655 ?
P1 K1 O3 K1 148.04(5) 1_665 . . 3_655 ?
P2 K1 O3 K1 -100.40(7) . . . 3_655 ?
O2 K1 O3 K1 154.14(4) 5_665 . . 7_667 ?
O1 K1 O3 K1 51.40(4) 7_667 . . 7_667 ?
O1 K1 O3 K1 -57.64(4) . . . 7_667 ?
O2 K1 O3 K1 63.87(7) 7_667 . . 7_667 ?
O5W K1 O3 K1 -132.93(4) 3_665 . . 7_667 ?
O3 K1 O3 K1 137.26(4) 5_665 . . 7_667 ?
O2 K1 O3 K1 -150.29(6) 3_665 . . 7_667 ?
O1 K1 O3 K1 -76.54(4) 3_665 . . 7_667 ?
O3 K1 O3 K1 0 7_667 . . 7_667 ?
P1 K1 O3 K1 177.60(3) 1_665 . . 7_667 ?
P2 K1 O3 K1 -70.85(2) . . . 7_667 ?
O3 Mn1 O4 C2 109.8(2) . . . . ?
O2 Mn1 O4 C2 -26.1(4) . . . . ?
O1 Mn1 O4 C2 -157.9(2) . . . . ?
O6 Mn1 O4 C2 13.3(2) . . . . ?
O5W Mn1 O4 C2 -72.8(2) . . . . ?
K1 Mn1 O4 C2 170.07(18) 7_667 . . . ?
K1 Mn1 O4 C2 -107.3(2) 5_565 . . . ?
K1 Mn1 O4 C2 71.5(2) 3_655 . . . ?
K1 Mn1 O4 C2 156.9(2) . . . . ?
O3 Mn1 O5W K1 -2.2(11) . . . 5_565 ?
O2 Mn1 O5W K1 48.07(6) . . . 5_565 ?
O1 Mn1 O5W K1 -47.54(6) . . . 5_565 ?
O4 Mn1 O5W K1 -143.63(6) . . . 5_565 ?
O6 Mn1 O5W K1 142.49(6) . . . 5_565 ?
K1 Mn1 O5W K1 -1.30(6) 7_667 . . 5_565 ?
K1 Mn1 O5W K1 65.77(6) 3_655 . . 5_565 ?
K1 Mn1 O5W K1 -67.32(6) . . . 5_565 ?
O3 Mn1 O6 C1 -110.7(2) . . . . ?
O2 Mn1 O6 C1 156.5(2) . . . . ?
O1 Mn1 O6 C1 25.6(4) . . . . ?
O4 Mn1 O6 C1 -13.3(2) . . . . ?
O5W Mn1 O6 C1 71.7(2) . . . . ?
K1 Mn1 O6 C1 -169.5(2) 7_667 . . . ?
K1 Mn1 O6 C1 107.3(2) 5_565 . . . ?
K1 Mn1 O6 C1 -158.8(2) 3_655 . . . ?
K1 Mn1 O6 C1 -73.4(2) . . . . ?
Mn1 O6 C1 O6 -168.8(3) . . . 10_557 ?
Mn1 O6 C1 C2 11.9(4) . . . . ?
Mn1 O4 C2 O4 168.6(2) . . . 10_557 ?
Mn1 O4 C2 C1 -11.9(4) . . . . ?
O6 C1 C2 O4 0.1(5) 10_557 . . 10_557 ?
O6 C1 C2 O4 179.5(2) . . . 10_557 ?
O6 C1 C2 O4 -179.5(2) 10_557 . . . ?
O6 C1 C2 O4 -0.1(5) . . . . ?

# The following lines are used to test the character set of files sent by
# network email or other means. They are not part of the CIF data set
# abcdefghijklmnopqrstuvwxyzABCDEFGHIJKLMNOPQRSTUVWXYZ0123456789
# !@#$%^&*()_+{}:"~<>?|\-=[];'`,./

# END of CIF
_exptl_crystal_recrystallization_method 'Hydrothermal synthesis'
_exptl_crystal_preparation       'Magnetic properties'
